# chap 5 solns - manual - materials...problem solutions introduction 5.1 briefly explain the...

Post on 20-May-2018

212 views

Embed Size (px)

TRANSCRIPT

CHAPTER 5

DIFFUSION

PROBLEM SOLUTIONS

Introduction

5.1 Briefly explain the difference between self-diffusion and interdiffusion.

Solution

Self-diffusion is atomic migration in pure metals--i.e., when all atoms exchanging positions are of the same

type. Interdiffusion is diffusion of atoms of one metal into another metal.

5.2 Self-diffusion involves the motion of atoms that are all of the same type; therefore it is not subject to

observation by compositional changes, as with interdiffusion. Suggest one way in which self-diffusion may be

monitored.

Solution

Self-diffusion may be monitored by using radioactive isotopes of the metal being studied. The motion of

these isotopic atoms may be monitored by measurement of radioactivity level.

Diffusion Mechanisms

5.3 (a) Compare interstitial and vacancy atomic mechanisms for diffusion.

(b) Cite two reasons why interstitial diffusion is normally more rapid than vacancy diffusion.

Solution

(a) With vacancy diffusion, atomic motion is from one lattice site to an adjacent vacancy. Self-diffusion and

the diffusion of substitutional impurities proceed via this mechanism. On the other hand, atomic motion is from

interstitial site to adjacent interstitial site for the interstitial diffusion mechanism.

(b) Interstitial diffusion is normally more rapid than vacancy diffusion because: (1) interstitial atoms, being

VP DOOHU DUH P RUH P RELOH DQG WKH probability of an empty adjacent interstitial site is greater than for a vacancy

adjacent to a host (or substitutional impurity) atom.

Steady-State Diffusion

5.4 Briefly explain the concept of steady state as it applies to diffusion.

Solution

Steady-state diffusion is the situation wherein the rate of diffusion into a given system is just equal to the

rate of diffusion out, such that there is no net accumulation or depletion of diffusing species--i.e., the diffusion flux is

independent of time.

5

.5 (a) Briefly explain the concept of a driving force.

(b) What is the driving force for steady-state diffusion?

Solution

(a) The driving force is that which compels a reaction to occur.

(b) The driving force for steady-state diffusion is the concentration gradient.

5.6

The purification of hydrogen gas by diffusion through a palladium sheet was discussed in Section 5.3.

Compute the number of kilograms of hydrogen that pass per hour through a 5-mm-thick sheet of palladium having

an area of 0.20 m

2

a t 500

C. Assume a diffusion coefficient of 1.0

10-

8 m

2/s, that the concentrations at the high-

and low-

pressure sides of the plate are 2.4 and 0.6 kg of hydrogen per cubic meter of palladium, and that steady-

state conditions have been attained.

Solution

This problem calls for the mass of hydrogen, per hour, that diffuses through a Pd sheet. It first becomes

necessary to employ both Equations 5.1a and 5.3. Combining these expressions and solving for the mass yields

M = JAt = - DAtDC

Dx

= - (

1.0

10

-8 m

2/s)(

0.20 m

2)

(3600 s/h)

0.

6 -

2.

4 kg /m

3

5

10-

3 m

= 2.6

10-

3 kg/h

5.7

A sheet of steel 1.5 mm thick has nitrogen atmospheres on both sides at 1200C and is permitted to

achieve a steady-state diffusion condition. The diffusion coefficient for nitrogen in steel at this temperatur

e is 6

10-

11 m

2

/s, and the diffusion flux is found to be 1.2

10-

7 kg/m

2-s. Also, it is known that the concentration of

nitrogen in the steel at the high-

pressure surface is 4 kg/m

3. How far into the sheet from this high-pressure side will

the concent

ration be 2.0 kg/m

3? Assume a linear concentration profile.

Solution

This problem is solved by using Equation 5.3 in the form

J = - DCA - CBxA - xB

If we take CA

to be the point at which the concentration of nitrogen is 4 kg/m

3, then it becomes necessary to solve

for xB, as

xB = xA + D CA - CB

J

Assume xA is zero at the surface, in which case

xB =

0 + (

6

10

-11 m

2/s)

4 kg /m

3 -

2 kg /m

3

1.

2

10-

7 kg / m

2 - s

= 1

10-

3

m = 1 mm

5.8

A sheet of BCC iron 1 mm thick was exposed to a carburizing gas atmosphere on one side and a

decarbur

izing atmosphere on the other side at 725C. After having reached steady state, the iron was quickly

cooled to room temperature. The carbon concentrations at the two surfaces of the sheet were determined to be

0.012 and 0.0075 wt%. Compute the diffusion

coefficient if the diffusion flux is 1.4

10-

8 kg/m

2-s. Hint: Use

Equation 4.9 to convert the concentrations from weight percent to kilograms of carbon per cubic meter of iron.

Solution

Let us first convert the carbon concentrations from weight percent to kilograms carbon per meter cubed

using Equation 4.9a. For 0.012 wt% C

CC" =

CCCCrC

+ CFerFe

10

3

=

0.

012

0.

012

2.

25 g/cm

3 +

99.

988

7.

87 g/cm

3

10

3

0.944 kg C/m

3

Similarly, for 0.0075 wt% C

CC" =

0.

0075

0.

0075

2.

25 g/cm

3 +

99.

9925

7.87 g/cm

3

10

3

= 0.590 kg C/m

3

Now, using a rearranged form of Equation

5.3

D = - J xA - xB

CA - CB

= - (

1.

40

10

-8 kg/m

2 - s) -

10-

3 m

0.

944 kg/m

3 -

0.590 kg/m

3

= 3.95

10-

11 m

2/s

5.9 When a-iron is subjected to an atmosphere of hydrogen gas, the concentration of hydrogen in the iron,

CH (in weight percent), is a function of hydrogen pressure,

pH

2 (in MPa), and absolute temperature (T)

according to

CH =

1.

34

10-

2 pH

2exp -

27.

2 kJ /mol

RT

(5.14)

Furthermore, the values of D

0 and Qd

for this diffusion system are 1.4

10-

7 m

2

/s and 13,400 J/mol, respectively.

Consider a thin iron membrane 1 mm thick t

hat is at 250C. Compute the diffusion flux through this membrane if

the hydrogen pressure on one side of the membrane is 0.15 MPa (1.48 atm), and on the other side 7.5 MPa (74

atm).

Solution

Ultimately we will employ Equation 5.3 to solve this problem. However, it first becomes necessary to

determine the concentration of hydrogen at each face using Equation 5.14. At the low pressure (or B) side

CH(B) = (

1.34

10

-2)

0.15 MPa exp -

27,

200 J/mo l

(

8.31 J/mol - K)(

250 +

273 K )

9.93

10-

6 wt%

Whereas, for the high pressure (or A) side

CH(A) = (

1.34

10

-2)

7.5 MPa exp -

27,

200 J/mol

(

8.31 J/mol - K)(

250 +

273 K )

7.02

10-

5 wt%

We now convert concentrations in weight percent to mass of nitrogen per unit volume of solid. At face B there are

9.93

10-

6

g (or 9.93

10-

9

kg) of hydrogen in 100 g of Fe, which is virtually pure iron. From the density of iron

(7.87

g/cm

3

), the volume iron in 100 g (VB) is just

VB =

100 g

7.

87 g /cm

3=

12.7 cm

3 =

1.27

10

-5 m

3

Therefore, the concentration of hydrogen at the B face in kilograms of H per cubic meter of alloy [

CH(B) ] is just

CH(B)'' =

CH(B)

VB

=

9.

93

10-

9 kg

1.

27

10-

5 m

3=

7.82

10

-4 kg/m

3

At the A face the volume of iron in 100 g (VA

) will also be 1.27

10-

5 m

3, and

CH(A)'' =

CH(A)

VA

=

7.

02

10-

8 kg

1.

27

10-

5 m

3=

5.53

10

-3 kg/m

3

Thus, the concentration gradient is just the difference between these concentrations of nitrogen divided by the

thickness of the iron membrane; that is

DC

Dx=

CH(B)'' - CH(A)

''

xB - xA

=

7.

82

10-

4 kg /m

3 -

5.

53

10-

3 kg /m

3

10-

3 m= -

4.75 kg/m

4

At this time it becomes necessary to calculate the value of the diffusion coefficient at 250

C using Equation 5.8.

Thus,

D = D

0 exp -QdRT

= (

1.

4

10-

7 m

2/s) exp -

13,

400 J/mol

(

8.31 J/mol - K)(

250 +

273 K)

= 6.41

10-

9 m

2/s

And, finally, the diffusion flux is computed using Equation 5.3 by taking the negative product of this diffusion

coefficient and the concentrat